**University of South Carolina**

**Scholar Commons**

Theses and Dissertations

2018

## Meso-Scale Simulation of Size-Dependent Shear

## Behavior in Glass Fiber Reinforced Polymer

## Reinforced Concrete Beams without Stirrups

Sina Khodaie

*University of South Carolina*

Follow this and additional works at:https://scholarcommons.sc.edu/etd Part of theCivil Engineering Commons

This Open Access Dissertation is brought to you by Scholar Commons. It has been accepted for inclusion in Theses and Dissertations by an authorized administrator of Scholar Commons. For more information, please contactdillarda@mailbox.sc.edu.

Recommended Citation

### M

ESO### -S

CALE### S

IMULATION OF### S

IZE### -D

EPENDENT### S

HEAR### B

EHAVIOR IN### G

LASS### F

IBER### R

EINFORCED### P

OLYMER### R

EINFORCED### C

ONCRETE### B

EAMS WITHOUT### S

TIRRUPSby Sina Khodaie Bachelor of Science

Sharif University of Technology, 2007 Master of Science

Sharif University of Technology, 2010

Submitted in Partial Fulfillment of the Requirements For the Degree of Doctor of Philosophy in

Civil Engineering

College of Engineering and Computing University of South Carolina

2018 Accepted by:

Fabio Matta, Major Professor Mohammed Alnaggar, Committee Member

Robert Mullen, Committee Member Paul Ziehl, Committee Member

© Copyright by Sina Khodaie, 2018 All Rights Reserved.

### DEDICATION

### ACKNOWLEDGMENTS

I would like to express my deepest appreciation to my advisor Dr. Fabio Matta for his passion, guidance, patience, and support as well as finding opportunities to fund my research. To my committee members: Dr. Mohammed Alnaggar, for productive discussions and providing guidance for the numerical simulations; Dr. Robert Mullen, for his support and belief in me during my PhD; and Dr. Paul Ziehl, for offering his advice and comments to improve my work. My gratitude also extends to my friends and fellow graduate students.

I would like to thank Dr. Gianluca Cusatis and Dr. Roozbeh Rezakhani for providing guidance for the numerical simulations. I would also like to thank Dr. Danielle Pelessone and Dr. Xinwei Zhou from Engineering and Software Systems Solutions (ES3) Inc. for providing excellent technical assistance with MARS Software.

I would like to acknowledge the research Cyberinfrastructure at USC for their assistance with the licensing and execution of MARS on the Maxwell cluster.

### ABSTRACT

There is extensive experimental evidence of the decrease in the shear stress at failure at increasing effective depths in concrete beams reinforced with glass fiber-reinforced polymer (GFRP) bars without shear reinforcement. An important practical implication is that extrapolating strength values from typical laboratory-scaled experiments to design larger members may be misleading. The complexity of the underlying mechanics is reflected in the difficulty of using commercially available numerical tools to accurately estimate shear strength irrespective of beam size. This dissertation presents research on a Lattice Discrete Particle Model (LDPM) based model to simulate the response of scaled slender GFRP reinforced concrete (RC) beams without stirrups. The numerical model includes: (1) a calibrated and validated concrete LDPM; (2) orthotropic GFRP bar elements; and (3) a nonlinear bond-slip law for the GFRP bar-concrete interface.

The second study presents a calibration and validation procedure for the concrete LDPM based on typical information available from reports on physical experiments (i.e., cylinder compressive strength, and maximum aggregate size). Next, the concrete LDPM implemented in the beam model is validated by accurately simulating the shear behavior of GRFP RC beams without stirrups having maximum aggregate size different from the first study, and effective depth in the range 146-292 mm where the size effect becomes evident.

In the third study, the influence of concrete fracture energy and maximum aggregate size are investigated numerically in two cases in which both the strength and failure mode of GFRP RC beams without stirrups are particularly difficult to predict. In fact. Based on the simulation results, it is recommended that fracture tests along with the compressive strength tests be performed on concrete specimens.

### TABLE OF CONTENTS

Dedication ... iii

Acknowledgements ... iv

Abstract ...v

List of Tables ...x

List of Figures ... xii

List of Symbols ... xvii

List of Abbreviations ... xxi

Chapter 1: Introduction ...1

1.1 Objective ...3

1.2 Scope ...4

1.3 References ...7

Chapter 2: Computation Simulation of Size-dependent Shear Behavior of Glass FRP Reinforced Concrete Beams without Stirrups...12

2.1 Introduction ...13

2.2 Load Tests ...17

2.3 Computational Framework ...18

2.4 Results and Discussion ...25

2.5 Concluding Remarks ...33

Chapter 3: Meso-scale Modeling of Shear Failure in

GFRP Reinforced Concrete Beams without Stirrups...55

3.1 Introduction ...55

3.2 Numerical Models of Concrete ...59

3.3 Computational Framework ...61

3.4 Calibration of LDPM Parameters ...65

3.5 Numerical Simulation of Load Tests ...72

3.6 Results and Discussion ...73

3.7 Conclusions ...78

3.8 References ...79

Chapter 4: Influence of Maximum Aggregate Size and Concrete Fracture Energy on Shear Response GFRP Reinforced Concrete Beams without Stirrups...100

4.1 Introduction ...101

4.2 Load Tests ...103

4.3 Computational Model ...104

4.4 Results and Discussion ...109

4.5 Conclusions ...115

4.6 References ...116

Chapter 5: Conclusions and Future Work ...134

Appendix A: Lattice Discrete Particle Modeling of Shear Failure in Scaled GFRP Reinforced Concrete Beams without Stirrups ...138

A.1 Introduction ...139

A.3 Calibration of LDPM Parameters ...144

A.4 Simulation of Load Tests on GFRP RC Beams ...150

A.5 Results and Discussion...151

A.6 Conclusions ...154

A.7 References ...154

Appendix B: Bond-Slip Law between GFRP Bars and Concrete ...169

Appendix C: Representative Input Files for Numerical Simulation of Four-Point Bending Load Tests ...177

C.1 Geometry Input File ...177

C.2 Beam Simulation Input File ...178

C.3 Failure Modeling of GFRP Bar Elements ...178

Appendix D: Experimental Results on Concrete Fracture Energy ...190

### LIST OF TABLES

Table 2.1 Experimental and analytical results of load tests ...41

Table 2.2 Concrete LDPM geometric parameters ...42

Table 2.3 LDPM meso-scale material parameters for Models A and B ...42

Table 2.4 Computational information on GFRP-RC beams load test simulations ...43

Table 2.5 Numerical results on GFRP-RC beams load test simulations ...43

Table 2.6 Contribution of shear transfer mechanisms at peak shear load ...44

Table 3.1 LDPM meso-scale geometric parameters ...89

Table 3.2LDPM meso-scale material parameters ...89

Table 3.3Computational information on the GFRP-RC beams simulations ...90

Table 3.4Experimental, analytical and LDPM-based results for GFRP-RC beams ...90

Table 4.1 Test matrix and experimental shear force at failure ...119

Table 4.2 Salient LDPM meso-scale parameters ...120

Table 4.3 Values of macroscopic mechanical properties of calibrated concrete models ...121

Table 4.4 Computational information for GFRP-RC beams simulations ...121

Table 4.5 Numerical results on contribution of shear transfer mechanisms at peak shear load in GS3 beam load tests ...122

Table 4.6 Numerical results for contribution of shear transfer mechanisms at peak load for S beams ...123

Table A.1 LDPM geometric parameters ...160

Table A.3 Specimen geometry for the tests ...161

Table A.4 Experimental and predicted shear strength ...161

Table B.1 Experimental results on GFRP bar-concrete bond properties ...172

### LIST OF FIGURES

Figure 1.1 Shear failure of 900 mm-deep beams

in Air Force Warehouse, Shelby, OH [2] ...10 Figure 1.2 (a) Collapse of the de la Concorde Overpass, in

Laval, Québec, Canada; and (b) shear crack in the

west abutment prior to failure ...11 Figure 2.1 Load tests: schematics of four-point-bending

load-test setup for scaled GFRPRC beam specimens

without stirrups, and cross sections. (Dimensions in mm.) ...45 Figure 2.2 Computational model: (a) shear crack in GFRP RC

beam and aggregate interlock with transfer of shear force, Vag, in concrete LDPM; (b) constitutive laws

for fracture in tension and tension-shear ...46 Figure 2.3 Numerical simulation of TPB test and

representative load-midspan displacement curve ...47 Figure 2.4 Uniaxial compression stress-strain

curves for calibrated models A and B ...47 Figure 2.5 (a) GFRP bar-concrete interaction; and (b)

experimental bond-slip envelope and adopted bond-slip law ...48 Figure 2.6 Representative schematics of test setup (S1 beam) ...48 Figure 2.7Results for S6 beams (d = 146 mm) using

Model A:(a) load-midspan deflection; (b) crack pattern at failure from experiments; and (c) evolution

of crack patterns from numerical simulations ...50 Figure 2.8Results for S3 beams (d = 292 mm) using

Model A: (a) load-midspan deflection; (b) crack pattern at failure from experiments; and (c) evolution

of crack patterns from numerical simulations ...49 Figure 2.9 Results for S1 beams (d = 883 mm) using

pattern at failure from experiments; and (c) evolution

of crack patterns from numerical simulations ...51 Figure 2.10 Maximum principal stress contour at peak load,

and distribution of axial and shear stress along the uncracked concrete ligament above the critical crack

in: (a) S6 beam; (b) S3 beam; and (c) S1 beam ...52
Figure 2.11 Evolution of crack width ratio, w*cr*/d*a*, at d/2 in S6, S3 and S1 beams ...53
Figure 2.12 Double logarithmic representation of size effect in S beams ...53
Figure 2.13 Evolution of shear transfer mechanism

contributions in (a) S6 beam, (b) S3 beam, and (c) S1 beam ...54 Figure 3.1 LDPM computational model: (a) random distribution

of aggregate particles within concrete volume; (b) outer mesh of specimen by assigning particle nodes to surfaces, edges and vertices; (c) twelve facets constructed within LDPM tetrahedron; (d) LDPM cell around aggregate particle; and (e) 2Drepresentation of potential

material failure regions within lattice system in beam section ...91 Figure 3.2 Computation modeling of aggregate interlocking

with transfer of shear force, V*ag*, along critical shear crack ...92
Figure 3.3 (a) GFRP bar-concrete LDPM tetrahedron interaction;

and (b) experimental bond-slip envelope and adopted model ...92 Figure 3.4 (a) Uniaxial compression: (a) stress-strain response

of concrete cylinders and calibrated concrete LDPM; (b) representative fracture pattern in experiments and

LDPM simulation...93 Figure 3.5 Flow chart for selection and calibration of LDPM material parameters ...94 Figure 3.6 Summary of the statistical results on total

fracture energy of concrete through TPB fracture tests ...95 Figure 3.7 Schematic of four-point bending test setup. (Dimensions in mm) ...95 Figure 3.8 Experimental and simulated load-midspan

deflection of (a) GS specimens; and (b) GM specimens ...96 Figure 3.9 Comparison of damage evolution between

different shear load, V: (a) GM1 specimen; and (b)

GS2 specimen. (Dimensions in mm.) ...97 Figure 3.10 Failure criterion along GFRP bar in GS beam at peak load ...98 Figure 3.11 Evolution of bond stress along

GM beam with increasing shear load, V ...98 Figure 3.12 Maximum principal stress contours in GS (top)

and GM (bottom) specimens at their peak shear load ...99 Figure 3.13 Representative stress states and maximum

principal stresses along critical crack in GM specimen ...99 Figure 4.1 Experimental results on GS1-3 specimens:

(a) load-midspan deflection curves; and (b) photographs

of specimens after failure (inset shows rupture of GFRP bar in GS2 beam) ...124 Figure 4.2 Four-point bending test setup and

cross sections of associated GFRP RC specimens ...125 Figure 4.3 Numerical simulation results for GS3-CM1

and GS3-CM5 models: (a) stress-strain curves from compression tests (markers point out compressive strength of tested cylinders); and

(b) load-midspan deflection curves from TPB fracture tests ...126 Figure 4.4 Load-midspan deflection results for GS3 specimen ...127 Figure 4.5 Crack patterns at failure from experiment (top)

and numerical simulations ...128 Figure 4.6 Maximum principal compressive stress

contours in GS3 beams at peak shear load...129 Figure 4.7 Load-midspan deflection results for S1 specimens ...130 Figure 4.8 Response of S1 beams: (a) experimental crack

patterns at failure; Numerical crack patterns at failure, maximum principal stress contour at peak load, and axial stress profile in uncracked concrete ligament above critical

Figure 4.9 Response of S6 beams: (a) load-midspan deflection results; numerical simulation response for (b) crack patterns

at failure; and (b) maximum principal stress contour at peak shear load ...132

Figure 4.10 Response of S3 beams: (a) load-midspan deflection results; numerical simulation response for (b) crack patterns at failure; and (b) maximum principal stress contour at peak shear load ...133

Figure A.1 LDPM cell around aggregate particle [23] ...162

Figure A.2 Uniaxial compression stress-strain response of concrete cylinders...162

Figure A.3 Uniaxial compression stress-strain curve for calibrated concrete LDPM...163

Figure A.4 Compression stress-strain response of
LDPM model as function of facet tensile strength, σ*t* ...163

Figure A.5 Compression stress-strain response of
LDPM model as function of tensile characteristic length, l*t* ...164

Figure A.6 Compression stress-strain response of
LDPM model as function of shear strength ratio, σ*s* /σ*t* ...164

Figure A.7 Typical fracture pattern for compression test in experiment and LDPM simulation. ...165

Figure A.8 Schematic of test setup ...165

Figure A.9 Schematics of simulated model ...162

Figure A.10 Experimental and simulated load-displacement response of GS specimens ...166

Figure A.11 Experimental and simulated load-displacement response of GM specimens ...166

Figure A.12 Simulation results of crack patterns in GM specimen for shear loads of 16 kN and 35 kN ...167

Figure A.13 Bond stress along bar in GM specimens ...167

Figure A.14 Bond stress along bar in GS specimens ...168

Figure B.2 Experimental envelope and adopted bond-slip law ...175

Figure B.3 Relevant bond-slip curves and bond strength values to load tests ... 176'

Figure C.1 MARS input file for GS3 specimen geometry and concrete LDPM tetrahedrons ...179

Figure C.2 Control parameters of simulation ...180

Figure C.3 GFRP material and bond-slip curve characteristics ...181

Figure C.4 Assigning material properties to concrete LDPM ...182

Figure C.5 Definition of GFRP bars and their contact model with concrete (f refers to shear stiffness multiplier for GFRP bars) ...183

Figure C.6 Definition of pinned supports ...184

Figure C.7 Definition of loading plate ...185

Figure C.8 Definition of displacement control loading ...186

Figure C.9 Time-history outputs for reaction at supports, midspan deflection, and energy quantities ...186

Figure C.10 Graphical output for displacements, stress tensors, and crack openings ...187

Figure C.11 MATLAB input file for reading axial and shear stress of GFRP bars and assigning bond stress ...188

### LIST OF SYMBOLS

*a * Coarse aggregate content (in concrete mix design) [mm]
*bw* Width of a beam specimen [mm]

*c * Cement content (in concrete mix design) [kg/m3]
*d * Effective depth of a beam [mm]

*da* Maximum aggregate size [mm]
*d*0 Minimum aggregate size [mm]

*D * Diameter of cylinder specimen [mm]
*eL* Shear strain in the facet

*eM* Shear strain in the facet
*eN* Normal strain in the facet
*E*0 Normal modulus [GPa]

*Ec* Elastic modulus of concrete [GPa]
*Ed * Densification ratio [GPa]

*Ef * longitudinal elastic modulus of GFRP bars [GPa]
*E*GFRP Elastic modulus of GFRP bars [GPa]

*EN* Normal elastic modulus of a facet [GPa]
*ET* Shear modulus of a facet [GPa]

*E*steel Elastic modulus of steel [GPa]

*f’cN * Numerical cylinder compressive strength of concrete [MPa]

*ffu* Average tensile strength of GFRP bars [MPa]
*Gf* Initial fracture energy [N/m]

*GF * Total fracture energy [N/m]

*G*GFRP Shear modulus of GFRP bars [GPa]

*G*steel Shear modulus of steel [GPa]

*Gt* Meso-scale fracture energy [N/m]
*Hc*0/E0 Initial hardening modulus ratio

𝓁 Inter-particle distance [mm]

*ld* Anchorage (development) length [mm]
*lt* Tensile characteristic length [mm]

**l** Normal unit vector of a local facet reference system [mm]
*L * Length of cylinder specimen [mm]

*m * Constant moment region length [mm]

**m** Transverse unit vector of a local facet reference system [mm]
*nt* Softening exponent

**n** Transverse unit vector of a local facet reference system [mm]
*s * Shear span of a beam [mm]

⟦**u***C*⟧ Displacement jump vector in a lattice strut [mm]

*V * Applied shear force [kN]

*Vc* Transmitted shear force through uncracked concrete [kN]
*Vd* Transmitted shear force through dowel action [kN]
*Ve* Experimental shear force at failure [kN]

*V*LDPM Numerically simulated shear capacity [kN]

*Vn* Nominal shear strength [kN]
*w * Water content in concrete [kg/m3_{] }

*wc* FPZ width [mm]

α Shear-normal coupling parameter

α0 Coefficient for round or angular aggregates

γ Coefficient of softening in bond stress-slip curve
δ*s* Slip between GFRP bar and concrete [mm]
ε*N* Normal strain in facet

ε*T* Shear strain in facet
η*F* Fuller coefficient
κ*c*0 Transitional strain ratio

κ*c*1 Deviatoric strain threshold ratio

κ*c*2 Deviatoric damage parameter

μ0 Initial friction

μ∞ Asymptotic friction

σ1 Axial stress in GFRP bars [MPa]

(σ1)*u* Ultimate axial stress in GFRP bars [MPa]
σ*c*0 Facet confined compressive strength [MPa]

σ*L* Shear stress in the facet (direction 1) [MPa]
σ*M* Shear stress in the facet (direction 2) [MPa]
σ*N* Normal stress in the facet [MPa]

σ*N*0 Transitional stress [MPa]

σ*s* Shear strength of the facet [MPa]
σ*s*/ σ*t* Shear strength ratio

σ*t* Tensile strength of the facet [MPa]
σ*T* Shear stress in facets [MPa]

σ*u* Ultimate tensile strength of GFRP bars [MPa]
σ*xx* Axial stress in concrete [MPa]

τ*b * Bond stress [MPa]

τ*f* Shear stress in GFRP bars [MPa]
(τf)*u* Shear strength of GFRP bars [MPa]
τ*xz * Shear stress in concrete [MPa]
υ Poisson’s ratio

### LIST OF ABBREVIATIONS

CHAPTER 1

### INTRODUCTION

Shear failure is considered one of the most critical failure modes for reinforced concrete (RC) structures, such as in the significant case of members without shear reinforcement. Different from other failure modes such as flexural failure, diagonal (shear) cracks form and propagate abruptly, indicating the onset of shear failure. The shear failure of RC members is usually catastrophic and needs to be accurately predicted and prevented.

Figure 1.2(a), resulting in five casualties. The collapse was due to the shear failure of the main bridge girders [3]. These examples demonstrate that the shear design algorithms may not always be effective in predicting the shear behavior of RC beams without stirrups.

Innovative materials have been introduced in the construction industry to enhance the performance of RC structures. For example, glass fiber reinforced polymer (GFRP) bars are being used as internal reinforcement in RC structures such as slab bridges, retaining walls, and sea walls [4] to eliminate the issue of corrosion. However, experimental evidence from load tests on scaled slender concrete (RC) beams internally reinforced with GFRP bars, and without stirrups, shows a significant decrease in the sectional shear stress at failure at increasing effective depths [5–7]. Existing nominal shear strength algorithms for GFRP RC structures are typically based on laboratory scaled specimens and extrapolation may be needed to obtain the nominal shear strength of large sized structures [6,8–11]. However, there are fundamental differences in describing the salient shear resisting mechanisms associated with the physical explanation of size effect among these approaches, as reviewed in chapter 2. In addition, there have been cases where such algorithms cannot consistently predict the shear strength and failure modes of GFRP-RC beams without stirrups, which demonstrates the difficulty of accurately accounting for the contribution of different shear transfer mechanisms, which largely depend on concrete fracture and friction behavior.

this end, it is desirable that candidate models account for concrete heterogeneity (i.e., role of aggregates and surrounding mortar), and incorporate constitutive laws that are relevant to simulate the size effect and salient shear resisting mechanisms. Among the candidate numerical models for concrete, which are reviewed in chapter 2, the Lattice Discrete Particle Model (LDPM) [12,13] was selected in this research to perform numerical simulations of four-point bending load tests on the GFRP-RC beams without stirrups, which were load tested as reported in the literature [6,14]. The LDPM is a discrete meso-scale concrete model that has the following attributes that are important to realistically simulate different shear resisting mechanisms, and the associated size effect: (1) it accounts for concrete heterogeneity by randomly placing aggregate particles with their actual size distribution within the specimen volume; and (2) it simulates shear-frictional cracking and aggregate interlocking in concrete by using discrete formulation and long-distance interactions between aggregate particles through lattice struts, along with incorporating vectorial constitutive laws for tension-softening and shear-friction behavior.

1.1 OBJECTIVE

reside: first, in providing a rational procedure for the calibration and validation of the
LDPM for concrete (which includes 21 meso-scale parameters) based on the minimal
information typically available from concrete mixture design and characterization tests
(i.e., cylinder compressive strength, *fc*, and maximum aggregate size, *da*); second, in the
implementation of an orthotropic GFRP bar model in the LDPM-based model as well as
an experimentally validated nonlinear bond-slip law; third, in capturing the size effect in
the shear strength of slender GFRP-RC beams without stirrups, and using the
computational results to investigate the contribution of salient shear transfer mechanisms
to the shear capacity; and fourth, in numerically investigating the effect of the concrete
fracture energy and maximum aggregate size on the response of such beams, and offering
conclusions and recommendations towards the development of accurate nominal shear
strength algorithms.

1.2SCOPE

The scope of the research is to address the objectives and novelties highlighted in the previous section and covered in chapters 2 through 4. In addition, four peer-reviewed papers published in the proceedings of international conferences are included as Appendices, providing pertinent information that complement the main body of this dissertation.

numerical simulations of three-point bending fracture tests based on RILEM standard specifications [15], compared to the literature-based estimate [16] driven from the reported maximum aggregate size, compressive strength, and water-cement ratio [6]. The computational simulations yielded accurate predictions of load-midspan deflection response, strength, crack patterns, and failure mode. The results provided insight into the contribution of the salient shear resisting mechanisms to shear capacity and size effect. The numerical simulation approach also highlighted the need for a rationale calibration procedure for the concrete LDPM when limited material characterization data are available (e.g., cylinder compressive strength), and the effect of the variations of concrete fracture energy as well as the aggregate size on the response of such beams need to be further investigated.

accurately estimate the load-deflection response, strength, and failure mode of the beams irrespective of size.

Chapter 4 presents a numerical study on the effect of concrete fracture energy
and maximum aggregate size on the response of GFRP-RC beams without stirrups under
four-point bending loading. Two significant cases are examined: (1) a specimen (GS3)
having effective depth, *d, equal to 146 mm, and nominal maximum aggregate size, da*,
equal to 6.3 mm, and two companion specimens (GS1 and GS2) with similar geometry
but nominal maximum aggregate size equal to 12.6 mm [14]; and (b) scaled GFRP RC
beams without stirrups denoted as S series (as described in chapter 2), having effective
depth in the range of 146-883 mm, and a constant maximum aggregate size equal to 19.1
mm [6]. The results highlight the importance of performing fracture tests, together with
standard compression tests, to more accurately model the fracture behavior of concrete,
and obtain better estimations of shear strength and failure modes.

Appendix A presents preliminary results on the calibration and validation of the LDPM parameters. Here, perfect bond between the GFRP bars and concrete is considered. The results suggest that this simplifying assumption fictitiously increases the shear strength of the beams and a nonlinear bond-slip law (as described in chapter 2) needs to be implemented, as done in the simulations presented in chapters 2 through 4.

Appendix C describes the input files for the geometric description of the concrete beams as well as the assembly and numerical simulation of four-point bending tests. In addition, the MATLAB code for the analysis of tensile and shear stresses in the GFRP bars is provided.

Appendix D presents the information for the fracture tests on concrete from the literature. The analysis of such data (e.g., Figure 3.6) provides information to determine the concrete fracture energy based on compressive strength, tensile strength, and maximum aggregate size.

1.3REFERENCES

[1] Wight JK. Reinforced Concrete Mechanics and Design. 7th edition. Pearson, London, UK; 2015.

[2] Lubell A, Sherwood T, Bentz E, Collins M. Safe Shear Design of Large Wide Beams. Concrete International 2004;26:66–78.

[3] Johnson PM, Couture A, Nicolet R. Commision of Inquirey into the Collapse of a Portion of the de la Concorde Overpass. Montreal, Quebec, CA: 2007.

[4] Matta F. Industry/university cooperative research on advanced composite reinforcement for concrete: translating innovation into sustainable engineering practice. Proc. US National Science Foundation International Workshop on the Use of Fiber Reinforced Polymers for Sustainable Structures, May 22, 2008, Cairo, Egypt, S.H. Rizkalla and A.-H. Hosny (Eds.), CD-ROM, 13 P.: 2008.

with FRP Reinforcement. Journal of Composites for Construction 2010;14:637– 46.

[6] Matta F, El-Sayed AK, Nanni A, Benmokrane B. Size Effect on Concrete Shear Strength in Beams Reinforced with Fiber-Reinforced Polymer Bars. ACI Structural Journal 2013;110:617–28.

[7] Cholostiakow S, Di Benedetti M, Guadagnini M, Zappa E. Shear behaviour of FRP RC beams: Does size matter? Proceedings of the 8th Biennial Conference on Advanced Composites in Construction, ACIC 2017, Sheffiled, U.K.: 2017, p. 6.

[8] ACI. Guide for the Design and Construction of Structural Concrete Reinforced with FRP Bars -American Concrete Institute (ACI 440.1R-15). Farmington Hills, MI: American Concrete Institute; 2015.

[9] CSA. Canadian Highway Bridge Design Code- CAN/CSA-S6-14. Mississauga, ON, Canada: 2014.

[10] Bažant ZP, Yu Q, Gerstle W, Hanson J, Ju JW. Justification of ACI 446 Code Provisions for Shear Design of Reinforced Concrete Beams. ACI Structural Journal 2007;104:601–10.

[11] Muttoni A, Ruiz MF. Shear Strength of Members without Transverse Reinforcement as Function of Critical Shear Crack Width. ACI Structural Journal 2008;105:163–72.

and Concrete Composites 2011;33:891–905.

[13] Cusatis G, Pelessone D, Mencarelli A. Lattice Discrete Particle Model (LDPM) for Failure Behavior of Concrete. I: Theory. Cement and Concrete Composites 2011;33:881–90.

[14] Matta F, Mazzoleni P, Zappa E, Sutton MA, Elbatanouny M, Larosche AK, et al. Shear Strength of FRP Reinforced Concrete Beams Without Stirrups : Verification

of Fracture Mechanics Formulation. ACI Special Publication 2012;286:1–14.

[15] RILEM. Determination of the fracture energy of mortar and concrete by means of three-point bend tests on notched beams. Materials and Structures 1985;18:285– 90.

**Figures: **

(a)

(b)

CHAPTER 2

### COMPUTATIONAL SIMULATION OF SIZE-DEPENDENT SHEAR

### BEHAVIOR OF GLASS FRP REINFORCED CONCRETE BEAMS

### WITHOUT STIRRUPS

ABSTRACT

2.1 INTRODUCTION

Shear failure in a slender reinforced concrete (RC) beam without stirrups typically occurs with the formation and propagation of an inclined crack via the combination of the flexural moment and shear force in the shear span. Shear forces in such beams are typically resisted by uncracked concrete in compression zone; through aggregate interlocking and tensile cohesive stresses along diagonal cracks; and dowel action in the longitudinal reinforcements [1]. Evidence from experimental load test on scaled slender RC beams without stirrups indicates a decrease in the nominal shear strength as the beam depth increases [2-5]. This phenomenon, known as size effect, is aggravated in beams that are internally reinforced with a similar amount of glass fiber reinforced polymer (GFRP) bars [6-9]. This occurs because the axial stiffness of GFRP bars is significantly (about 80%) lower than that of conventional steel bars. Consequently, in practice, extrapolating the shear strength of large structures such as slab bridges, retaining walls, and seawalls based on the results of the laboratory tested specimens may be misleading [9,10].

The fracture mechanics-based shear strength algorithm proposed by ACI committee 446 [14], which is also applicable to GFRP-RC beams once the smaller axial stiffness of the reinforcement is accounted for [9], acknowledges the role of transferred shear force along the critical shear crack (i.e., aggregate interlock) along with the major role of the uncracked concrete in shear-compression to the shear capacity. This approach explains the size effect based on the ratio of fracture process zone (FPZ) to the depth of uncracked concrete ligament above the critical shear crack, where shear-compression and cohesive stresses are transferred. Because of the constant size of the FPZ, increasing the effective depth decreases such ratio, resulting in a more localized compressive stress profile due to compression softening, and thus a smaller sectional shear strength [15].

The modified compression field theory (MCFT) [16], which is implemented in the Canadian code [17] and the AASHTO LRFD bridge design specifications [18], provides the fundamental basis for a nominal shear strength algorithm that enables one to estimate the shear strength of steel and GFRP-RC structures. Here, size effect is attributed to the decrease in the contribution of aggregate interlock as the primary means of shear transfer, as the beam effective depth increases (e.g., [7]).

The different physical explanations of size effect in the aforementioned shear strength algorithms highlight a knowledge gap in accurately accounting for the contribution of different shear transfer mechanisms and their interplay, which are mainly governed by concrete fracture and frictional behavior.

Different numerical models of RC concrete beams simulated the size effect by incorporating the strain softening behavior of concrete in tension and shear-compression, and the frictional behavior, into their constitutive laws [22-25]. The crack band model [26] has been implemented in concrete models to address the fracture behavior of concrete. An et al. [22] described the loss of shear stress transfer along the shear cracks by decreasing the concrete shear stiffness as a function of the strain normal to the crack opening. Červenka and Papanikolaou [23] considered a plasticity model with softening

for concrete under shear-compression stresses. They also related the shear stiffness of the cracked concrete to the normal crack opening law. Syroka-Korol et al. [24] assigned non-local softening behavior in tension and compression in the concrete constitutive laws and performed size effect simulations discounting the shear force transfer through aggregate interlock mechanism. Bažant and Caner [25] proposed the microplane model for concrete

localized on planes with different orientations (microplanes) within each element, which is representative of cracking and damage within concrete; and (3) it benefits from strain dependent yield boundaries (rather than scalar hardening-softening parameters) that facilitates realistic simulation of concrete under large deformations.

Ideally, a candidate numerical model of concrete to simulate the shear transfer mechanisms, and provide accurate predictions of shear strength, must account for the concrete heterogeneity along with the fracture and frictional response. To this end, the Lattice Discrete Particle Model (LDPM) [27,28], which shares its fundamental concepts with the microplane model (i.e., presenting potential material failure planes and vectorial constitutive laws), is considered in this dissertation. The LDPM is a meso-scale concrete model (i.e., includes aggregates and mortar) that has the following characteristics that are important to realistically simulate different shear resisting mechanisms, and the associated size effect: 1) it accounts for concrete heterogeneity by randomly placing aggregate particles with their actual size distribution from the mix design; 2) it enables the simulation of mixed mode fracture and the associated cracking to capture aggregate interlocking due to the discrete formulation, mechanical interaction between the aggregates, and the implementation of fracture and shear-frictional constitutive laws; and 3) it enables the simulation of strut-and-tie behavior of concrete leading to tensile fracture under unconfined compressive stresses.

criterion, and a nonlinear bond-slip for the GFRP bar-concrete interface. Preliminary research presented evidence on the accurate simulation of shear behavior of GFRP-RC beams without stirrups with effective depth in the range 146-292 mm [29]. Here, physically representative computational simulations of shear behavior of slender GFRP-RC beams without stirrups having effective depth in the range 146-883 mm, and exhibiting size effect in the range of 50-65%, are presented and discussed. The analysis of the simulation results offers an insight toward understanding the role of different shear transfer mechanisms and their interplay.

2.2 LOAD TESTS

The cross sections and four-point-bending load test setup for the scaled GFRP
RC beam specimens are illustrated in Figure 2.1. The specimens include small size
companion specimens S6-0.12-2A and S6-0.12-3A, having an effective depth *d = 146 *
mm, medium size companion specimens S3-0.12-1A and S3-0.12-2, having d = 292 mm,
and large size companion specimens S1-0.12-1A and S1-0.12-2B, having *d = 883 mm *
[9]. These specimens valid candidates to study the size effect, since specimens S3 and S6
were designed to scale their effective depth by one-third and one-sixth, respectively, with
respect to the S1 counterparts, while maintaining constant shear span-to-effective depth
ratio, *s/d, of 3.1, effective reinforcement ratio, ρeff*, of 0.12%, and maximum aggregate
size, d*a*, of 19.1 mm. Table 2.1 summarizes salient information including: effective depth,

*d; shear span-to-depth ratio s/d; concrete cylinder compressive strength, fc*; average

*Vb*; and nominal shear capacity, V*n*, based on the ACI 440 [11], modified ACI 446 [9,14],
refined (second-order) MCFT [30], and CSCT [19] algorithms.

From Table 2.1, it is noted that the predictions of shear strength based on existing algorithms, often tend to be more conservative for the smaller beams, and tend to be closer to the test results as the beam effective depth increases [9]. This evidence highlights the difficulty of reflecting salient shear resisting mechanisms and their interplay, and thus accurately predicting shear strength irrespective of size.

2.3 COMPUTATIONAL FRAMEWORK

This section presents the components of the computational framework that is used to simulate the load tests on the scaled GFRP-RC beams without stirrups. The components include the LDPM concrete model, the GFRP bar model, and the GFRP bar-concrete interface model.

2.3.1 Concrete

2.3.1.1 Lattice Discrete Particle Model

fracture are based on the crack band model [26] which allows transfer of tensile cohesive
stresses along the inclined cracks where tensile and shear stresses are generated. In fact,
normal tensile stress-strain, σ*N* - ε*N*, and shear stress-strain, σ*T* – ε*T*, responses of the facets
are plotted in Figure 2.2b. Here, different σ*N* - ε*N* and σ*T* – ε*T* curves are characterized for
each fact based on the value of the coupling variable, ω, which represents the degree of
interaction between normal and shear loading, transitioning from pure tension (ω = π/2)

to pure shear (ω = 0). Through definition of the LDPM constitutive laws, a smooth transition is provided from softening behavior in pure tension to perfectly plastic behavior in pure shear as presented in the case of ω = π/8 in Figure 2.2b where both

tensile and shear stresses are present in the facets. Thus, the generated shear stresses in the diagonal cracks, increase the width of the band where tensile cohesive stresses are transferred along the crack.

2.3.1.2 Meso-scale parameters

The LDPM parameters for the concrete used in all beams (i.e., S6, S3, and S1) are selected based on the following criteria:

• Geometric parameters, which determine the geometry of concrete

meso-structure, are reflective of the actual mixture design of the concrete from each load tested beam [9].

• Material parameters, which describe the LDPM constitutive laws for concrete

elastic and inelastic behavior, are obtained so that the concrete models yield to similar concrete cylinder compressive strength obtained from the experiments, and their fracture energy, GF, is well within the range 80-100 N/m which is reasonable for normal strength concrete as highlighted in the literature (e.g., [32-34]).

Based on the available information for the concrete on the load tested beams,
the geometric and material parameters for concrete models A (for S6 and S3 beams) and
B (for S1 beam) are presented in Tables 2.2 and 2.3, respectively. The information on the
concrete included concrete cylinder compressive strength, *fc*, and maximum aggregate
size, d*a*. The procedure for calibrating the concrete model is as follows.

First, the geometric parameters are determined based on the typical mixture
design. Here, minimum aggregate size, *d*0, controls the resolution of the model and is

usually designated so that at least 20% of the aggregate volume is modeled [28].

experimental results, the parameter σ*s* /σ*t*, which is the ratio of the shear strength to the
tensile strength in the facets, is adjusted. σ*s* /σ*t* is the predominant factor in defining the

strength limit of the facets in tension and shear [27], and thus greatly influences the
macroscopic compressive strength of concrete, f’*c*, where mixed mode fracture in tension

and shear is the dominant failure mechanism [35].

Third, the salient fracture related meso-scale parameters, tensile strength, σ*t*,
and tensile characteristic length, *lt*, are calibrated so that the concrete model yields a
suitable *GF* through simulations of three-point bending (TPB) tests according to RILEM
[36]. Tension-softening constitutive laws are defined by σ*t* and l*t* specifying the maximum
tensile stress and tensile softening modulus of the facets in pure tension. These
parameters along with the inter-particle distance (related to the maximum aggregate size)
affect the macroscopic tensile strength and the total fracture energy, *GF*, of the concrete.
In particular, by controlling the softening modulus in the facet stress-strain curves, σ*t* and
*lt* influence the width of the FPZ. Figure 2.3 illustrates the numerical simulation setup
along with representative concrete crack pattern and load-displacement curve. Here,
multiplying the area under the curve by the ligament area provides numerical value of G*F*
for the concrete. The TPB fracture tests were not performed in the experimental
campaign with the beam load tests. However, *GF* can be estimated based on the typical
information provided for concrete (i.e., cylinder compressive strength, *fc*, maximum
aggregate size, *da*, and water-cement ratio, *w/c) using a formula by Bažant and *
Becq-Giraudon [32]:

###

###

0.46###

0.22###

0.30

2.5 0.051 1 11.27

*F* *c* *a*

where α0 is equal to 1 and 1.44 for rounded and angular aggregates, respectively. Based

on the available information for the concrete used for the load tested beams [9], the
estimated G*F* assuming round and crushed aggregates for the concrete used for the S6 and
S3 beams is 73 N/m and 106 N/m, respectively. Hence, the fracture parameters of Model
A are calibrated so that the numerical simulation of TBP tests yields *GF* = 89 N/m.
Following the same procedure for the concrete used for the S1 beams having *fc* = 29.5
MPa, Model B with G*F* = 87 N/m is calibrated. It is noted that variations of concrete G*F*
affect the FPZ width near the crack tip and the shear-compression band in uncracked
concrete above the critical shear crack. Thus, it may change the contribution as well as
the interplay of the shear transfer mechanisms, and thus influence both shear strength and
size effect [26].

point, no further parameter changes were performed, and the concrete LDPM models were used in the numerical simulation of the load tests.

2.3.2 GFRP Reinforcement Model

Pultruded E-glass/vinyl ester GFRP bars were used as internal reinforcement in the beam specimens [9]. These bars are made of anisotropic composite materials that exhibit a linear elastic behavior in tension up to a brittle failure. The bars have higher tensile strength compared to the conventional steel bars, but their elastic and shear modulus are significantly lower. To simulate such behavior, the finite elements are formulated based on the Mindlin-Reissner [37] plate theory, in which a stiffness multiplier equal to 0.36 was applied to the isotropic shear modulus to yield the designated shear modulus. In four-point bending load tests, the activation of the dowel action mechanism in the shear span puts the GFRP bars under combined tensile and shear stresses. For this reason, the Tsai-Hill failure criterion [38] is considered to address the multiaxial tensile and shear stresses that contribute to failure:

###

###

2 2

1

*f* *f*

*f*

*f* _{u}_{u}

_{} _{}

_{} _{}

(2.2)

2.3.3 GFRP Bar-concrete Interaction Model

of the adjacent LDPM tetrahedron as illustrated in Figure 2.4a. The behavior of these
nonlinear springs is described by the bond-slip law obtained from pull-out tests and beam
tests for GFRP bars embedded in concrete. Here, the modified
Bertero-Popov-Eligehausen (BPE) model was implemented to describe the bond-slip law [39] in the
LDPM-based numerical simulations. The selected bond-slip model consists of an
ascending branch associated with chemical bond, friction due to surface roughness, and
mechanical bonding followed by a softening branch due to the loss of the mechanical
bond, and a residual frictional strength. This model effectively evaluates the bond-slip
response at the GFRP bar-concrete interface [40]. Figure 2.4b shows the adopted
bond-slip law, together with the envelope of bond-bond-slip diagrams, representative curves, and
peak bond stress markers from the relevant experimental pull-out and beam tests [41-45].
This model was obtained by averaging the experimental data available in the literature
and including factors such as concrete compressive strength, *f’c*, and bar diameter, and
surface treatment of the GFRP bars.

2.3.4 Numerical Simulation of Load Tests

4. The numerical simulations were executed through explicit dynamic algorithm and using displacement control loading procedure, in which the loading plate moved at the constant rate of 4 cm/s. Convergence of the simulation was achieved by using a maximum time step of 1×10-6 s. The ratio of the kinetic energy to the internal work during the simulation was monitored and found to be less than 1%, which confirmed that dynamic effects of the loading rate were minimal and quasi-static state of loading was attained during the numerical simulations.

2.4 RESULTS AND DISCUSSION 2.4.1 Structural Response and Size Effect

Salient data obtained through the simulations are summarized in Table 2.4,
where: *V*LDPM is the simulated shear strength; *V*LDPM/(b*wdfc*0.5) is the normalized shear
strength; ΔVLDPM /(b*wdfc*0.5) is the change in the normalized shear strength with respect to
the S6 beam; σ*f* and τ*f* are the axial and shear stress in the GFRP bars at the location of

the diagonal crack in the shear span at the peak load; and, *wcr* is the crack width at *d/2 *
from the top of the beam at the peak load.

2.4.1.1 S6 specimens (scale 1:6)

mode was attained at the failure load equal to 86% of the load associated with the flexural load through the numerical simulations. In fact, as presented in Table 2.5, the failure index of the GFRP bar based on Tsai-Hill criterion is equal to 0.91 indicating its impending rupture in tension-shear capacity similar to the response obtained in the experiments for S6-0.12-2A specimen [9]. It is noted that, although the S6-0.12-3A specimen failed in diagonal tension, its shear capacity is still 17-62% above the predicted values from the nominal shear strength algorithms presented in Table 2.1. The relatively lower attained shear strength could be attributed to the particular diagonal crack passing through relatively smaller aggregates which reduced the contribution of aggregate interlocking [47], and resulted in a narrower FPZ width due to the smaller inter-particle distance [15].

2.4.1.2. S3 specimens (scale 1:3)

still maintains a residual strength, which diminishes as the critical shear crack becomes wider and the failure occurs subsequently at the instance III.

2.4.1.3. S1 specimens (scale 1:1)

For the S1 beams, fairly accurate estimates of shear load-midspan deflection
in pre- and post-cracking regions, as well as the evolution of the crack patterns are
obtained by the numerical simulations, as illustrated in Figure 2.9. Here, a brittle failure
instantly occurred with the formation and propagation of the critical shear crack towards
the loading plate. In line with the results from the experiments [9], the size effect in the
numerically simulated normalized shear strength of the S1 beam was 30% and 65%, with
respect to the S3 and S6 beams, respectively. The Tsai-Hill failure index for the S1 beam
is 0.24 indicating the shear failure with minimal damage to the GFRP bars. The
maximum shear crack width, w*cr*,max, in the S1 beam at the peak load reached 17.2 mm,

which is 90% of *da*, implying minimal transferred cohesive stresses and aggregate
interlock mechanisms that explains the lack of residual resistance from the beam after
propagation of the critical shear crack in the compression zone leading to the immediate
failure.

contribution of different shear transfer mechanisms and their interplay at different loading stages up to failure.

2.4.2 Shear Force Resisting Mechanisms

The components of macroscopic stress tensor are acquired in each LDPM cell
by summing up the contribution of all the facets through application of principle of
virtual work (i.e., equating the total internal work of the facets with the external work in
each LDPM cell) [27]. Figure 2.10 presents the maximum principal stress contours,
along with the axial stress, σ*xx*, and the shear stress, τ*xz*, profiles in the uncracked concrete

ligament above the critical shear crack at the peak shear load in the S6, S3, and S1 beams. Within the shear spans, areas with compressive (negative) principal stresses highlight the regions where the shear forces are resisted. These areas of tensile fracture, occurring along the critical shear crack, and shear-compression fracture, occurring above such a crack, are of particular interest. Here, the negative maximum principal stress is resultant of the exerted compressive axial stresses and shear stresses in the concrete, which are generated in the uncracked concrete above the critical shear crack, diagonal crack fronts where aggregate interlocking develops, and the GFRP-concrete interface at the location of the diagonal cracks where dowel action develops.

Table 2.6 summarizes the contribution of the salient shear transfer
mechanisms to the shear capacity at the peak load. Here, as presented in Figure 2.10, an
average shear stress, τ*xz*, profile is assessed for the concrete ligament above the critical

GFRP bar to its cross section at the intersection of the critical crack. Lastly, the transferred shear forces along the critical shear crack (through aggregate interlock mechanism) consist of the remainder of the total shear force.

2.4.2.1 Uncracked Concrete Above the Critical Crack

Based on the simulation results, in all specimen sizes, shear forces are primarily resisted by the uncracked concrete above the critical shear crack subjected to shear-compression stresses. In fact, inclined compressive stresses through the uncracked concrete ligament above the critical shear crack transmit 68% of the shear capacity in the S6 and S3 beams, and their contribution increased to 86% of the shear capacity in the S1 beams.

The contribution of the uncracked concrete to the normalized shear strength
decreased by 0.074 MPa0.5 (50%) and 0.082 MPa0.5 (56%), in the S3 beams (having d =
292 mm) and the S1 beams (having d = 883 mm) compared to the S6 beams (having d =
146 mm), respectively. This result is associated with the size effect in the
shear-compression fracture of the concrete above the critical shear crack [15]. Since the salient
characteristics of the concrete used in all the specimens are similar (i.e., f*c* ≈ 30 MPa, G*F*
≈ 86 N/m, and *da* = 19 mm), the effective width of the shear-compression band, in line

fact, the uncracked concrete depth-to-effective depth ratio decreased from 0.3 in the S6 beam, to 0.23 and 0.18 in the S3 and S1 beams, respectively.

2.4.2.2 Aggregate interlock

The contribution of the aggregate interlock to the shear capacity is significant
in the small to medium size beams (i.e., S6 and S3 beams). This is due to the relatively
smaller crack width (5.7 mm and 8.2 mm for S6 and S3 beams, respectively) in such
beams that allows the activation of aggregate interlocking until the failure of the
specimen. According to Table 2.6, the contribution of the aggregate interlocking in the S6
and S3 beams is equal to 28% and 29% of the shear capacity, respectively. However, in
the S1 beam with *d = 883 mm, the maximum crack width is equal to 17.2 mm, and the *
contribution of the aggregate interlocking is only 10% of the shear capacity.

Although the aggregate interlock is the secondary means for the transfer of
shear forces, its contribution to the size effect is significant. In fact, the normalized shear
strength decreased by 0.03 MPa0.5 (49%) and 0.053 MPa0.5 (87%), in the S3 beams and
the S1 beams compared to the S6 beams, respectively. This reduced contribution is
attributed to the wider width of the shear cracks in the larger beams through which less
shear forces were transferred [47]. This aspect is represented in Figure 2.11, in which the
evolution of the shear crack width-to-maximum aggregate size ratio, *wcr*/d*a*, with respect
to the increased normalized shear stresses is plotted. The maximum of *wcr*/d*a* increases
from 0.3 in the S6 beam to 0.9 in the S1 beam.

of the critical shear crack at 49% of the peak load, its normalized shear strength is gradually increased. Instead, in the S3 beam, and particularly S1 beam, the aggregate interlock is activated close to the peak load of the beams (i.e., 92% and 95% of the peak load for the S3 beam and S1 beams, respectively) and the failure of the beams occur immediately. This transition can be compared to the asymptotes in size effect law proposed by Bažant et al. [14] presented in Figure 2.12. According to this law, in a small

structure, the FPZ occupies a large portion of the cross section and the failure behavior is closer to plastic limit analysis, in which the strength limit is reached simultaneously in most of the failure surface. This type of failure is associated with the asymptote equal to zero for the exponent of the power law. In a larger structure, the FPZ occupies a smaller portion of the cross section; i.e., it is more localized. Therefore, the response is closer to that predicted by linear elastic fracture mechanics (LEFM) which is associated with the asymptote equal to -1/2 for the exponent of the power law. Here, for the smaller beams (in particular, the S6 beams), because of significant effect of the aggregate interlock to the shear capacity, the scatter of the experimental data is larger. However, the brittle response of the S1 beam is accurately represented by the LEFM asymptote. This highlights an important characteristic of the size effect law in predicting the shear capacity of the extremely large structures based on the LEFM asymptote, where extrapolation of the experimental data is needed.

2.4.2.3 Dowel action

GFRP bars. Although, a size effect equal to 66% is also seen in the contribution of the dowel action between the S1 and S6 beams, its relatively negligible magnitude (0.006 MPa0.5) renders this mechanism as the less significant one for the size effect.

2.4.2.4 Evolution of shear transfer mechanisms

Based on the provided results regarding to the cases presented in this paper, both mechanisms including uncracked concrete above the critical shear crack, as well as the aggregate interlocking along such crack contribute to size effect on the shear strength of GFRP RC beams without stirrups. Therefore, any mechanics-based numerical model attempting to simulate the size effect in shear, must represent both shear resisting mechanisms faithfully.

mechanisms and their interplay at the level of service load in the beams which can assist researchers and practitioners in the damage evaluation of the existing structures.

In line with the findings in this paper, the finite element simulations conducted
by Bažant and Yu [15], demonstrated that in the small beams (i.e., *d *< 300 mm), the

crack bridging stresses have a significant contribution to the shear capacity of the RC beams without stirrups. But in larger beams (i.e., d > 1000 mm) their relative contribution is decreased, as the majority of the shear load is transmitted through inclined compressive stresses above the critical shear crack. It is noted that the geometry of the specimens as well as the reinforcement material in those simulations were different. However, similar trend in the contribution of the shear transfer mechanisms to the size effect is observed.

2.5 CONCLUDING REMARKS

Computational models of GFRP RC beams without stirrups, and with effective depth ranging from 146 mm to 883 mm, were developed. The model included a calibrated and validated concrete LDPM based on the available information from the experiments [9] and literature, an orthotropic GFRP bar material model, and an experimentally validated nonlinear bond-slip law for GFRP bar-concrete interfaces. The following conclusions were drawn:

• The proposed computational modelling approach, which considers the fracture

• The shear forces transferred through the uncracked concrete above the critical

shear crack, and along such crack (i.e., aggregate interlock), contribute to shear capacity and size effect. The uncracked concrete is the predominant medium for providing the beam strength (68%-86% in S6 and S1 beams). However, aggregate interlock plays a major role on size effect with a 87% decrease in the normalized shear strength at increasing effective depth from 146 mm to 883 mm. With decreasing contribution of aggregate interlock, failure of the GFRP RC beams without stirrups becomes mode abrupt, which is typically the case for large members.

• Dowel action provided a negligible contribution to the shear strength.

• A robust calibration procedure needs to be introduced for the case where only *fc*

and *da* are known, which is the typical case in research and practice. For an
accurate prediction of shear strength, it is recommended that fracture tests be
performed along with standard compression tests to characterize concrete.

2.6 REFERENCES

[1] Wight JK. Reinforced Concrete Mechanics and Design. 7th Edition. Pearson, London, UK; 2015.

[2] Kani GNJ. How Safe are Our Large Reinforced Concrete Beams. ACI Journal Proceedings 1967;64:128–41.

[3] Bažant, Z. P., Kazemi MT. Size Effect on Diagonale Shear Failure of Beams without Stirrups. ACI Jouranl 1991;88:268–76.

[5] Collins MP, Kuchma D. How Safe Are Our Large, Lightly RC Beams, Slabs, and Footings? ACI Structural Journal 1999;96:482–90.

[6] Tureyen AK, Frosch RJ. Shear tests of FRP-reinforced concrete beams without stirrups. ACI Structural Journal 2002;99:427–34.

[7] Bentz EC, Massam L, Collins MP. Shear Strength of Large Concrete Members with FRP Reinforcement. Journal of Composites for Construction 2010;14:637– 46.

[8] Alam MS, Hussein A. Effect of Member Depth on Shear Strength of Polymer – Reinforced Concrete Beams 2012:119–26.

[9] Matta F, El-Sayed AK, Nanni A, Benmokrane B. Size Effect on Concrete Shear Strength in Beams Reinforced with Fiber-Reinforced Polymer Bars. ACI Structural Journal 2013;110:617–28.

[10] Matta F, Mazzoleni P, Zappa E, Sutton MA, Elbatanouny M, Larosche AK, et al. Shear Strength of FRP Reinforced Concrete Beams Without Stirrups :

Verification of Fracture Mechanics Formulation. ACI Special Publication 2012;286:1–14.

[11] ACI Committee 440. Guide for the Design and Construction of Structural Concrete Reinforced with FRP Bars, ACI 440.1R-15. American Concrete Institute, Farmington Hills, MI: 2015.

[13] Tureyen AK, Frosch RJ. Concrete Shear Strength: Another Perspective. ACI Structural Journal 2003;100:609–15.

[14] Bažant ZP, Yu Q, Gerstle W, Hanson J, Ju JW. Justification of ACI 446 Code Provisions for Shear Design of Reinforced Concrete Beams. ACI Structural Journal 2007;104:601–10.

[15] Bažant ZP, Yu Q. Designing Against Size Effect on Shear Strength of Reinforced Concrete Beams Without Stirrups: II. Verification and Calibration. Journal of Structural Engineering 2005;131:1886–97.

[16] Vecchio FJ, Collins MP. The Modified Compression-Field Theory for Reinforced Concrete Elements Subjected to Shear. ACI Journal 1986;83:219–31.

[17] CAN/CSA-S6-14. Canadian Highway Bridge Design Code. Canadian Standard Association, Mississauga, ON, Canada: 2014.

[18] AASHTO. AASHTO LRFD Bridge Design Specifications. 8th edition, American Association of State Highway and Transportation Officials, Washington, D.C.: 2017.

[19] Muttoni A, Ruiz MF. Shear Strength of Members without Transverse Reinforcement as Function of Critical Shear Crack Width. ACI Structural Journal 2008;105:163–72.

[20] Swiss Society of Engineers and Architects. SIA Code 262 for Concrete Structures. Zürich, Switzerland: 2003.

[22] An X, Maekawa K, Okamura H. Numerical Simulation of Size Effect in Shear Strength of RC Beams. Journal of Materials, Concrete Structures and Pavement, JSCE 1997;35:297–316.

[23] Červenka J, Papanikolaou VK. Three Dimensional Combined Fracture-Plastic Material Model for Concrete. International Journal of Plasticity 2008;24:2192– 220.

[24] Syroka-Korol E, Tejchman J, Mróz Z. FE analysis of size effects in reinforced concrete beams without shear reinforcement based on stochastic elasto-plasticity with non-local softening. Finite Elements in Analysis and Design 2014;88:25–41. [25] Caner FC, Bažant ZP. Microplane Model M7 for Plain Concrete. I: Formulation.

Journal of Engineering Mechanics 2013;139:1714–23.

[26] Bažant ZP, Oh B. Crack Band Theory for Fracture of Concrete. Materials and Structures 1983;16:155–77.

[27] Cusatis G, Pelessone D, Mencarelli A. Lattice Discrete Particle Model (LDPM) for Failure Behavior of Concrete. I: Theory. Cement and Concrete Composites 2011;33:881–90.

[28] Cusatis G, Mencarelli A, Pelessone D, Baylot J. Lattice Discrete Particle Model (LDPM) for Failure Behavior of Concrete. II: Calibration and Validation. Cement and Concrete Composites 2011;33:891–905.

[30] Hoult NA, Sherwood EG, Bentz EC, Collins MP. Does the Use of FRP Reinforcement Change the One-Way Shear Behaviour of Reinforced Concrete Slabs? Journal of Composites for Construction 2008;12:125–33.

[31] Ceccato C, Salviato M, Pellegrino C, Cusatis G. Simulation of Concrete Failure and Fiber Reinforced Polymer Fracture in Confined Columns with Different Cross Sectional Shape. International Journal of Solids and Structures 2017;108:216–29.

[32] Bažant ZP, Becq-Giraudon E. Statistical Pprediction of Fracture Parameters of Concrete and Implications for Choice of Testing Standard. Cement and Concrete Research 2002;32:529–56.

[33] Rosselló C, Elices M, Guinea GV. Fracture of Model Concrete: 2. Fracture Energy and Characteristic Length. Cement and Concrete Research 2006;36:1345– 53.

[34] Hoover CG, P. Bažant Z, Vorel J, Wendner R, Hubler MH. Comprehensive Concrete Fracture Tests: Description and Results. Engineering Fracture Mechanics 2013;114:92–103.

[36] RILEM. Determination of the fracture energy of mortar and concrete by means of three-point bend tests on notched beams. Materials and Structures 1985;18:285– 90.

[37] Reissner E. The Effect of Transverse Shear Deformation on the Bending of Elastic Plates. Journal of Applied Mechanics 1945;12:69–77.

[38] Kaw AK. Mechanics of Composite Materials. CRC Press, Boca Raton, FL; 2005. [39] Cosenza E, Manfredi G, Realfonzo R. Behavior and Modeling of Bond of FRP

Rebars to Concrete. Journal of Composites for Construction 1997;1:40–51.

[40] Lin X, Zhang YX. Evaluation of Bond Stress-slip Models for FRP Reinforcing Bars in Concrete. Composite Structures 2014;107:131–41.

[41] Ehsani MR, Saadatmanesh H, Tao S. Bond Behavior of Deformed GFRP Rebars. Journal of Composite Materials 1997;31:1413–30.

[42] Tighiouart B, Benmokrane B, Gao D. Investigation of Bond in Concrete Member with Fibre Reinforced Polymer (FRP) Bars. Construction and Building Materials 1998;12:453–62.

[43] Focacci F, Nanni A, Bakis C. Local Bond-slip Relationship for FRP Reinforcement in Concrete. Journal of Composites for Construction 2000;4:24– 31.

[44] Benmokrane B, Tighiouart B, Chaallal O. Bond Strength and Load Distribution of Composite GFRP Reinforcing Bars in Concrete. ACI Materials Journal 1996;93:246–53.

[46] ES3. MARS Manual, Version 2017.06.27. Engineering and Software System Solutions, Inc. 2017.

**Tables: **

Table 2.1Experimental and analytical results of load tests

Specimen *d *
[mm]
*fc*
[MPa]
*E*GFRP
[GPa]
*ffu*
[MPa]
*Ve*
[kN]
*e*
*w* *c*
*V*

*b d* *f*

[ MPa ]

*Vb *

[kN]

*Vn* [kN]

ACI 440 [11] ACI 446 [9] Hoult et al. [30] CSCT [18] S6-0.12-2A

146 3.1

32.1 43.2 849 36.9 0.195 48.5 10.1 18.6 19.0 21.9

S6-0.12-3A 32.1 43.2 849 26.3 0.139 48.5 10.1 18.6 19.0 21.9

S3-0.12-1A

292 3.1

32.1 43.2 849 19.2 0.102 48.5 10.1 16.1 17.7 16.4

S3-0.12-2A 32.1 43.2 849 17.9 0.095 48.5 10.1 16.1 17.7 16.4

S1-0.12-1A

883 3.1

29.5 41.0 476 154 0.070 348 117 132 163 117

S1-0.12-2B 29.6 41.0 483 151 0.069 353 117 133 163 117

**s**

**d**

4

Table 2.2 Concrete LDPM geometric parameters

Geometric parameters Models

A and B
Cement mass content, *c* [kg/m3_{] } _{389 }

Water-to-cement ratio, *w*/*c* 0.45

Aggregate-to-cement ratio, *a*/*c* 5.2

Maximum aggregate size, *da* [mm] 19

Fuller coefficient, η*F* 0.45

Minimum aggregate size, *d*0 [mm] 11

Table 2.3 LDPM meso-scale material parameters for Models A and B

Material parameters Model A Model B

Normal modulus, *E*0 [GPa] 36 36

Shear-normal coupling parameter, α 0.24 0.24

Tensile strength, σ*t* [MPa] 3.1 2.8

Shear strength ratio, σ*s*/σ*t* 4.1 4.7

Tensile characteristic length, *lt* [mm] 180 170

Softening exponent, *nt* 0.2 0.2

Initial friction, μ0 0.2 0.2

Transitional stress, σ*N*0 [MPa] 600 600
Confined compressive strength, σ*c*0 [MPa] 100 100

Densification ratio, *Ed* 1 1

Initial hardening modulus ratio, *H*c0/*E*0 0.4 0.4

Transitional strain ratio, κ*c*0 2 2

Deviatoric strain threshold ratio, κ*c*1 1 1

Deviatoric damage parameter, κ*c*2 5 5